Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

PRL 112, 034301 (2014) week ending 24 JANUARY 2014 PHYSICAL REVIEW LETTERS Ï FIG. 2 (color online). Schematics of wave propagation direction with respect to interfacial layers. FIG. 1 (color online). Schematics of undeformed and deformed periodic multilayered structures with interfacial phase volume fractions (a) cÃ°iÃ Â¼ 0.02 and (b) 0.04. (c) Dependence of stress vs strain and wrinkle amplitude vs strain. The stress-strain results are given by the continuous black (cÃ°iÃ Â¼ 0.04) and red curves (cÃ°iÃ Â¼ 0.02); the dashed curve is the solution for flat layers, assuming no wrinkling. The dotted curves represent the evolution of the normalized wrinkle amplitude (right axis). The stiffness ratio of the phases is Î¼Ã°iÃ =Î¼Ã°mÃ Â¼ 100. Here, we analyze the propagation of elastic waves in finitely deformed periodic materials. To this end, we consider incremental small-amplitude motions superimposed on a finitely deformed state [20]. Differently from a plane wave, a wave propagating in a periodic structure is the superposition of plane waves, which can be described by the Bloch function [1,23]. Consequently, the smallamplitude motions are implemented in terms of Bloch waves ui Ã°x; tÃ Â¼ Ui Ã°x; tÃ expÃ°ik Â· xÃ, where ui is the displacement, k is the Bloch vector and Ui is a periodic function subjected to the periodicity condition U i Ã°x; tÃ Â¼ Ui Ã°x Ã¾ a; tÃ with a being a lattice translation vector [12,20,23]. To perform this analysis, we use the finite element method, which allows us (i) to obtain the solution for the deformed periodic composite after the bifurcation, and (ii) then superimpose the Bloch-Floquet periodicity condition on the deformed state and solve the eigenvalue problem associated with the wave equations. For completeness, the numerical solution was verified against exact analytical solutions for finitely deformed infinite homogeneous and layered materials, and excellent agreement was found. We define the direction of wave propagation via angle Ï as shown in Fig. 2. The influence of interface wrinkling on wave propagation is shown in Fig. 3 which compares the dispersion diagrams for (a) the undeformed state, where the applied strain Ïµ Â¼ 0, to (b) those at the onset of wrinkling formation Ïµ â Ïµcr , and to (c) those for a developed wrinkled state Ïµ > Ïµcr . Figure 3 shows examples of dispersion diagrams for various composites with different stiffness ratios rÎ¼ Â¼ Î¼Ã°iÃ =Î¼Ã°mÃ : different density contrast ratios rÏ Â¼ ÏÃ°iÃ =ÏÃ°mÃ , and different interfacial layer volume fractions of cÃ°iÃ to allow comparison pï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬ï¬of these effects. The normalized frequency Ï~ Â¼ Ïh ÏÃ°mÃ =Î¼Ì is reported. The dispersion diagram of the undeformed structure appears in the top row. The composites present in columns (1)â(3) and (4) exhibit elastic instabilities at different levels of critical strain, in particular, at Ïµcr Â¼ 0.040 08 and Ïµcr Â¼ 0.0086, respectively. Consequently, we present the dispersion diagrams for these cases at different strain levels (middle rows), namely at Ïµ Â¼ 0.04 for composites in columns (1)â(3) and Ïµ Â¼ 0.01 for column (4). Finally, we show the dispersion diagrams for a developed wrinkled state in the bottom row for strains of Ïµ Â¼ 0.048 for composites in columns (1)â(3), and Ïµ Â¼ 0.017 for column (4). For composites present in columns (1) and (2), the normalized amplitudes of the wrinkles are A~ Â¼ 0.2687 and 0.5075 at Ïµ Â¼ 0.04 and 0.048, respectively. The corresponding amplitudes for the composite (3) are 0.271 and 0.524, respectively. For the composite (4), the amplitudes of the wrinkles are A~ Â¼ 0.522 and 1.058 at Ïµ Â¼ 0.01 and 0.017, respectively. The dispersion diagrams show different branches of wave propagation including transverse and longitudinal waves. In our analysis, we specifically focus on identifying complete band gaps, when both, longitudinal and transverse waves, cannot propagate. The undeformed composite does not filter waves in a direction along the interface at any frequency; however, the deformed composites with wrinkled interfaces exhibit clear band gaps [see columns (1), (2), and (4) in line (b)]. The frequency range of the band gaps is denoted by the grey filled area in Fig. 3. Note that one-dimensional phononic crystals with flat layers can never prevent wave propagation parallel to the layers [24]. In contrast, the wrinkled interfaces introduce variations of the mechanical properties in the direction of wave propagation, and, consequently, secondary waves are generated. The waves interfere with each other such that for some combination of the material properties, 034301-2

Similar